Synthesis and characterization of CuO nanowires by a simple wet chemical method
© Ethiraj and Kang; licensee Springer. 2012
Received: 13 September 2011
Accepted: 5 January 2012
Published: 5 January 2012
We report a successful synthesis of copper oxide nanowires with an average diameter of 90 nm and lengths of several micrometers by using a simple and inexpensive wet chemical method. The CuO nanowires prepared via this method are advantageous for industrial applications which require mass production and low thermal budget technique. It is found that the concentration and the quantity of precursors are the critical factors for obtaining the desired one-dimensional morphology. Field emission scanning electron microscopy images indicate the influence of thioglycerol on the dispersity of the prepared CuO nanowires possibly due to the stabilization effect of the surface caused by the organic molecule thioglycerol. The Fourier transform infrared spectrum analysis, energy dispersive X-ray analysis, X-ray diffraction analysis, and X-ray photoemission spectrum analysis confirm clearly the formation of a pure phase high-quality CuO with monoclinic crystal structure.
Since the discovery of carbon nanotubes, the synthesis of one-dimensional morphology such as nanowires and nanorods has gained much attention because this constitutes an important building block of nanodevices and integrated nanosystems [1–5]. Among the available transition metal oxides, such as Ni, Cu, Zn, and Fe, synthesis of CuO is an important topic of research. Cupric oxide, CuO, which is a p-type semiconductor [6, 7] (indirect bandgap of 1.2 to 1.5 eV) has been widely exploited for diverse applications, such as an active electrode material for Li-ion batteries, field emission [FE] emitters, heterogeneous catalysts, gas sensors, and solar cells [8–13]. Moreover, the evidence of a spin-dependent quantum transport phenomenon in CuO nanowires was already reported . Till now, many methods have been developed to synthesize CuO nanowires or nanorods, such as thermal oxidation of copper foil, hydrothermal route, aqueous reaction, vapor-liquid-solid synthesis, solution-liquid-solid synthesis, laser ablation, arc discharge, precursor thermal decomposition, electron beam lithography, and template-assisted synthesis [5, 15–19]. However, all these methods either require high temperatures, sophisticated instrumentation, inert atmosphere, or long reaction time. The difference between the method in this manuscript and the aqueous reaction referred earlier is the starting precursor material used and the stabilizer. In our case, the precursor used is copper acetate, while in the aqueous reaction, copper chloride. We used the organic molecule thioglycerol [TG] as stabilizer, while no stabilizer was used in the latter case.
Moreover, until now, few reports are available in literature for the synthesis of CuO nanowires using the organic molecule TG. Therefore, in the present study, a systematic effort has been made to synthesize CuO nanowires by a simple and inexpensive wet chemical method using copper acetate and NaOH as the precursor material in the presence of organic molecule TG. The possible formation mechanism of CuO nanowires via this chemical method is also discussed.
All the reagents were of analytical grade and were used without further purification. Copper acetate [(CH3COO)2-H2O] and sodium hydroxide [NaOH] were used as precursors in the present experiment. Two separate solutions, copper acetate (0.5 M) in deionized [DI] water and NaOH (5 M) in DI water, were prepared. Aqueous copper acetate and aqueous NaOH solutions were referred to as solution A and solution B, respectively. Stirring is continued until the respective metal salts are completely dissolved in DI water. Later 1 μL of TG is added to solution A, and the solution is stirred for a few minutes. Solution B is then added to the reaction mixture, and water is immediately added. Further stirring continued for a few minutes. Centrifugation is done to collect the precipitate. Washing of the precipitate is carried out using the DI water for five to six times. Finally, the collected precipitate is dried overnight at 35°C.
The morphology of the CuO nanowires obtained in the present work was investigated by a field emission scanning electron microscope [FE-SEM] (JEOL JSM-7401F; JEOL Ltd., Akishima, Tokyo, Japan) operated at an accelerated voltage of 10 kV. The energy dispersive X-ray analysis [EDX] was carried out on the scanning electron microscopy [SEM] system. X-ray diffraction [XRD] spectra of the CuO samples were obtained using a powder X-ray diffractometer (D8 FOCUS 2200 V Bruker AXS, Bruker Optik Gmbh, Ettlingen, Germany), using Cu Kα radiation (λ = 1.5418 Å) with 2θ ranging from 20° to 80°. The Fourier transform infrared spectrum [FTIR] of CuO samples in the form of pellets was recorded using a Perkin Elmer 1615 spectrometer (PerkinElmer, Waltham, MA, USA). Pellets were prepared by mixing CuO powder with KBr, and spectrum was recorded in the range of 400 to 4,000 cm-1. X-ray photoelectron spectroscopy [XPS] measurements were performed on ESCA MK II (VG Scientific Ltd., London, England) set up by using an Al Kα X-ray source (hν = 1486.6 eV). All the experiments were carried out at a base pressure of approximately 10-9 mbar, and a C 1s spectrum at 285.0 ± 0.2 eV served as the internal reference.
Results and discussion
When the reaction in Equation 1 proceeds with the nucleation and crystal growth, the Gibbs free energy of the nanocrystallite surfaces is very high, and in order to decrease the Gibbs free energy, the nanocrystallites tend to aggregate . Therefore, the flower morphology of CuO is obtained. However, when a small amount of TG is introduced in the synthesis of CuO, instead of a flower morphology, well-dispersed CuO nanowires are obtained, which can be speculated due to the stabilization effect caused by the use of organic molecule TG. Moreover, the role of TG is different from what structure-directing agents such as CTAB and HMTA are doing. In our case, without any structure-directing agent, we are able to generate CuO nanoflowers. When we carried out the CuO synthesis using TG, we obtained only separated CuO nanowires which clearly imply that the role of TG is definitely different from the role of CTAB and HMTA, where use of these agents leads to some kind of morphological changes in the material formation. Hence, the role of TG in our case is just for dispersion due to surface stabilization. An in-depth study is required, and further experiments are underway to understand and investigate the exact mechanism and the role of TG in the synthesis of CuO nanowires.
In order to detect the elements present in the CuO samples, EDX analysis was carried out. The spectrum (not shown) indicates the presence of copper [Cu], oxygen [O], and silicon [Si]. No other impurity was detected. The presence of Si was from the substrate. Thus, the formation of CuO was confirmed from the EDX.
Using a simple and inexpensive wet chemical method, the synthesis of copper oxide nanowires with diameters of 90 nm and lengths of several micrometers has been successfully carried out. The concentration and quantity of precursors are the critical factors for obtaining the desired 1-D morphology. SEM micrographs clearly indicate the influence of TG on the dispersity of the prepared CuO nanowires which may be due to the stabilization effect of the surface caused by the organic molecule TG. The FTIR and XPS data analyses confirm the formation of a pure phase CuO with monoclinic crystal structure. EDX and XRD data support the same finding.
This work was supported by the Korea Science and Engineering Foundation (KOSEF) and the National Research Foundation of Korea (NRF) grants funded by the Korean government (KRF-2006-311-C00050), R31-2008-000-10029-0 (World Class University Program), and 2011-0011775 (Basic Science Research Project).
- Patzke GR, Krumeich F, Nesper R: Oxidic nanotubes and nanorods-anisotropic modules for a future nanotechnology. Angew Chem Int Ed 2002, 41: 2446–2461. 10.1002/1521-3773(20020715)41:14<2446::AID-ANIE2446>3.0.CO;2-KView Article
- Dekker C: Carbon nanotubes as molecular quantum wires. Phys Today 1999, 52: 22.View Article
- Huang Y, Duan XF, Cui Y, Lauhon LJ, Kim KH, Lieber CM: Logic gates and computation from assembled nanowire building blocks. Science 2001, 294: 1313–1317. 10.1126/science.1066192View Article
- Hu J, Odom TW, Lieber CM: Chemistry and physics in one dimension: synthesis and properties of nanowires and nanotubes. Acc Chem Re 1999, 32: 435–445. 10.1021/ar9700365View Article
- Martel R, Schmidt T, Shea HR, Hertel T, Avouris P: Single-and multi-wall carbon nanotube field-effect transistors. Appl Phys Lett 1998, 73: 2447–2449. 10.1063/1.122477View Article
- Marabelli F, Parravicini GB, Salghetti-Drioli F: Optical gap of CuO. Phys Rev B 1995, 52: 1433–1436. 10.1103/PhysRevB.52.1433View Article
- Fan H, Yang L, Hua W, Wu X, Wu Z, Xie S, Zou B: Controlled synthesis of monodispersed CuO nanocrystals. Nanotechnology 2004, 15: 37–42. 10.1088/0957-4484/15/1/007View Article
- Switzer JA, Kothari HM, Poizot P, Nakanishi S, Bohannan EW: Enantiospecific electrodeposition of a chiral catalyst. Nature 2003, 425: 490–493. 10.1038/nature01990View Article
- Anandan S, Wen X, Yang S: Room temperature growth of CuO nanorod arrays on copper and their application as a cathode in dye-sensitized solar cells. Mater Chem Phys 2005, 93: 35–40. 10.1016/j.matchemphys.2005.02.002View Article
- Chowdhuri A, Sharma P, Gupta V, Sreenivas K, Rao KV: H2S gas sensing mechanism of SnO2films with ultrathin CuO dotted islands. J Appl Phys 2002, 92: 2172–2180. 10.1063/1.1490154View Article
- Bennici S, Gervasini A: Catalytic activity of dispersed CuO phases towards nitrogen oxides (N2O, NO, and NO2). Appl Catal B 2006, 62: 336–344. 10.1016/j.apcatb.2005.09.001View Article
- Ghosh S, Avasthi DK, Shah P, Ganesan V, Gupta A, Sarangi D, Bhattacharya R, Assmann W: Deposition of thin films of different oxides of copper by RF reactive sputtering and their characterization. Vacuum 2000, 57: 377–385. 10.1016/S0042-207X(00)00151-2View Article
- Hsieh CT, Chen JM, Lin HH, Shin HC: Field emission from various CuO nanostructures. Appl Phys Lett 2003, 83: 3383–3385. 10.1063/1.1619229View Article
- Gillingham DM, Müller C, Hong J, Wu RQ, Bland JAC: Evidence of spin-dependent quantum transport effects in CuO nanowires. J Phys Cond Matter 2006, 18: 9135–9142. 10.1088/0953-8984/18/39/039View Article
- Kaur M, Muthe KP, Despande SK, Choudhury S, Singh JB, Verma N: Growth and branching of CuO nanowires by thermal oxidation of copper. J Cryst Growth 2006, 289: 670–675. 10.1016/j.jcrysgro.2005.11.111View Article
- Cao MH, Wang YH, Guo CX, Qi YJ, Hu CW, Wang EB, Nanosci J: A simple route towards CuO nanowires and nanorods. Nanotech 2004, 4: 824–828.
- Wang WZ, Varghese OK, Ruan CM, Paulose M, Grimes CA: Synthesis of CuO and Cu [sub 2] O crystalline nanowires using Cu (OH)[sub 2] nanowire templates. J Mater Res 2003, 18: 2756–2759. 10.1557/JMR.2003.0384View Article
- Xu C, Lin Y, Xu G, Wang G: Preparation and characterization of CuO nanorods by thermal decomposition of CuC2O4precursor. Mater Res Bull 2002, 37: 2365–2372. 10.1016/S0025-5408(02)00848-6View Article
- Jiang XC, Herricks T, Xia YN: CuO nanowires can be synthesized by heating copper substrates in air. Nano Lett 2002, 2: 1333–1338. 10.1021/nl0257519View Article
- Zhang H, Yang D, Ji Y, Ma X, Xu J, Que D: Low temperature synthesis of flowerlike ZnO nanostructures by cetyltrimethylammonium bromide-assisted hydrothermal process. J Phys Chem B 2004, 108: 3955–3958. 10.1021/jp036826fView Article
- Gao X, Li X, Yu W: Flowerlike ZnO nanostructures via hexamethylenetetramine-assisted hermolysis of zinc-ethylenediamine complex. Phys Chem B 2005, 109: 1155–1161. 10.1021/jp046267sView Article
- Ethiraj AS, Hebalkar N, Kulkarni SK, Pasricha R, Dem C, Schmitt M, Kiefer W, Weinhardt L, Joshi S, Fink R, Heske C, Kumpf C, Umbach E: Enhancement of photoluminescence in manganese-doped ZnS nanoparticles due to a silica shell. J Chem Phys 2003, 118: 8945–8953. 10.1063/1.1566932View Article
- Khosravi AA, Kundu MM, Kuruvilla BA, Shekhawat GS, Gupta RP, Sharma AK, Vyas PD, Kulkarni SK: Manganese doped zinc sulphide nanoparticles by aqueous method. Appl Phys Lett 1995, 67: 2506–2508. 10.1063/1.114440View Article
- Zhu J, Chen H, Liu H, Yang X, Lu L, Wang X: Needle-shaped nanocrystalline CuO prepared by liquid hydrolysis of Cu(OAc)2. Mater Sci and Eng 2004, A 384: 172–176.View Article
- Zhu J, Bi H, Wang Y, Wang X, Yang X, Lu L: Synthesis of flower-like CuO nanostructures via a simple hydrolysis route. Mater Lett 2007, 61: 5236–5238. 10.1016/j.matlet.2007.04.037View Article
- Wang JZ, Xu J, Zhu J, Chen HY: Preparation of CuO nanoparticles by microwave irradiation. J Cryst Growth 2002, 244: 88–94. 10.1016/S0022-0248(02)01571-3View Article
- Nyquist RA, Kagel RO: Infrared Spectra of Inorganic Compounds. New York and London: Academic Press; 1997:220.
- Kliche K, Popovic ZV: Far-infrared spectroscopic investigations on CuO. Phys Rev B 1990, 42: 10060–10066. 10.1103/PhysRevB.42.10060View Article
- Zheng L, Liu X: Solution-phase synthesis of CuO hierarchical nanosheets at near-neutral pH and near-room temperature. Mater Lett 2007, 61: 2222–2226. 10.1016/j.matlet.2006.08.063View Article
- Moulder J, Sticke W, Sobol P, Bomben K: Standard ESCA spectra of the elements and line energy information. In Handbook of X-ray Photoelectron Spectroscopy. Edited by: Chastain J. USA: Perkin Elmer Coorporation: Physical Electronics Division; 1992.
- Hong ZS, Cao Y, Deng JF: A convenient alcohothermal approach for low temperature synthesis of CuO nanoparticles. Mater Lett 2002, 52: 34–38. 10.1016/S0167-577X(01)00361-5View Article
- Zarate RA, Hevia F, Fuentes S, Fuenzalida VM, Zuniga A: Novel route to synthesize CuO nanoplatelets. J Solid State Chem 2007, 180: 1464–1469. 10.1016/j.jssc.2007.01.040View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.